Article Type : Research Article

Authors : Run Xu, Boyong Hur, Hyojun An and Jiaguang Liu

Keywords : Super plasticity; Behavior; Stress; Parameters; Material

Three parameters are
discussed in this paper. It is found that the superplastic behavior happens in
the condition of m=0.6, n=0.09 & K=240MPa. It fits well to formula and
m>K>n too in above paper. With decreasing K and n and increasing m the
strain will become low to benefit super plastic behavior to happen.
??(K=(?^(1/?) ) ? ) Is a formula to be adopted to super plasticity, here
suppose n=1/e. This expresses well the superplastic behavior.

The super plasticity is a
new approach to gain the biggest super plasticity to satisfy all the demand in
material industry. In current the research is developing positively to metals
and inorganic materials. The main conditions affect it is micro grains besides
low strain rate and temperature [1,2]. In this paper it is modeled that the
relationship among stress sensitive exponents m? strength coefficient K and
stress exponent n is observed. On the other hand a modeling from elongation
convergence is applied to look for the super plasticity. It is found that the
super plasticity will happen at 300% elongation from its convergence. It is a
new find for super plasticity approach method from pure mathematics. These
three parameters are discussed to confirm the relationship among them for us to
continue to last find m>K>n [3]. TiAl super plasticity will happen at the
conditions of low strain rate (<5×10-4/s) and temperature (>1298K) [4].
So in this paper is adopted that the value in literature above is to model and
analyze further study. Overview the parameter is investigated to consider their
relationships in order to find the clear factor effectiveness to high strain
and elongation. For instance the K-m, K-n and K-stress all they can be found
through curve and formulas to look for precision relations of them. The final
aim will be known the large elongation condition upon them relations. To try to
check the key and subordination effective factor for super plasticity approach
and find internal deep relation according to detail classification and analogue
is this study ultimate aim and destination.

Since the Three parameters are discussed in this paper. It is found that the superplastic behavior happens in the condition of m=0.6, n=0.09& K=240MPa. It fits well to formula and m>K>n too in above paper. With decreasing K and n and increasing m the strain will become low to benefit super plastic behavior to happen. is a formula to be adopted to super plasticity, here suppose n=1/e which can be concept from reference [2]. This expresses well the superplastic behavior according to the Figure 1(b). As it is known that there is a summit that arrives 300MPa stress then it curve down to long strain. The lowest one with K=240MPa is near superplastic behavior from the curve that lasts 2000% strain which is dominant super plasticity. The middle one is K=340MPa whose summit arrives 500MPa while the largest is K=440MPa whose summit arrives 600MPa from the Figure 1.

(a) n

(b)K

(c) m&K2

*Figure
1:** The relationship between flow stress *

So K=240MPa is the best
condition for super plasticity which may be less than K=300MPa some. The
reasonable region is less than 300MPa as K=240MPa. It is difficult to gain the
good plasticity when K=440MPa. It expresses low strain will be attained under
this condition. Here K is parameter and ? is stress. From m<K<n relation
K is second factor to affect the stress but when it is proposed that n=1/? the
result becomes better than original K. so reverse is reasonable to express the
phenomenon of super plasticity. The reverse ? is meaning in this study
dominantly as literature [2] expresses

As seen in (a~b) the m is weaker parameter totally than the n and m has more increasing trend while n is reasonable with their differences. Here we find the little m and n to cause lower stress that expresses the elongation is good. However the little descending stress is found in (a) that expresses the stability result is created while m causes continuous descending one. Moreover the little stress like 300MPa is good one it explains little stress can make the fine elongation up to 700% strain value. So the n has stable trend than the m here. It is usual that the stability has easily control method than the descending one. So it is concluded that K>n>m is found in this study that is some different result than literature [2] whose turn is m>K>n in terms of . As seen in Figure 1(c) two parameters has been checked and found the optimum one is m=0.6; K2=202 meantime one of m=0.302;K2=202 is high. It expresses that m=0.6 is good one. Overview the big n and m will affect K to small one that causes the small stress directly and gains big strain.

Three parameters are discussed
in this paper and it is found that the superplastic behavior happens in the
condition of m=0.6, n=0.09& K=240MPa. It fits well to formula and
m>K>n too in reference paper. With decreasing K and n and increasing m
the strain will become low to benefit super plastic behavior to happen.

- Zhang K, Chen G, Wang G. Superplasticity
in Ceramics J Inorganic Mat. 2003; 18: 707.
- Run Xu. Convergence Proving of the
Theoretical and True Elongation Inequalities by Derivation and Analogy. J
Metallic Mat Res. 2020; 3: 15-17.
- Run Xu. Model for Superplastic Deformation of Ti3Al Alloys. Int J Plant Engineering and Management. 2019; 24: 251-254.
- Zhang J, Xu Y, Huang B. Study on deformation
Dynamics behaviors of superplasticity in TiAl base alloys. Rare Metal Materials
and Engineering. 2014; 43: 1493-1494.

SunText Reviews Content is available under Commons Attribution 4.0 License Copyright © 2021 suntextreviews.org - All Right Reserved